| ||Format||Pages||Price|| |
|6||$54.00||  ADD TO CART|
|Hardcopy (shipping and handling)||6||$54.00||  ADD TO CART|
|Standard + Redline PDF Bundle||12||$64.00||  ADD TO CART|
Significance and Use
5.1 The pull-off strength of a bonded FRP system is an important performance property that has been used in specifications, particularly those for assessing the quality of an application. This test method serves as a means for uniformly preparing and testing bonded FRP systems, and evaluating and reporting the results.
5.2 Variations in results obtained using different devices are possible. Therefore, it is recommended that the type of adhesion test device (including manufacturer and model) be mutually agreed upon between the interested parties.
5.3 This test method is intended for use in both the field and the laboratory.
5.4 The basic material properties obtained from this test method can be used in the control of the quality of adhesives and in the theoretical equations for designing FRP systems for external reinforcement to strengthen existing structures.
1.1 This test method describes the apparatus and procedure for evaluating the pull-off strength of wet lay-up or pultruded (shop-fabricated) Fiber Reinforced Polymer (FRP) laminate systems adhesively bonded to a flat concrete substrate. The test determines the greatest perpendicular force (in tension) that an FRP system can bear before a plug of material is detached. Failure will occur along the weakest plane within the system comprised of the test fixture, FRP laminate, adhesive, and substrate.
1.2 This test method is primarily used for quality control and assessment of field repairs of structures using adhesive-applied composite materials.
1.3 This test method is appropriate for use with FRP systems having any fiber orientation or combination of ply orientations comprising the FRP laminate.
1.4 This test method is appropriate for use with flat concrete, concrete masonry, clay masonry, and stone masonry substrates.
1.5 This test method is not appropriate for use as an “acceptance” or “proof” wherein the FRP system remaining intact at a prescribed force is an acceptable result.
1.6 Pull-off strength measurements depend upon both material and instrumental parameters. Different adhesion test devices and procedures will give different results and cannot be directly compared.
1.7 This test method can be destructive. Spot repairs may be necessary. The test method will result in an exposed cut FRP section; repair methods must consider the potential for moisture uptake through this cut section.
1.8 Prior to the installation of some adhesively bonded FRP systems, the substrate must be patched. This test method is not appropriate for determining the pull-off strength of the FRP from the patch material. An additional test method is required to determine the pull-off strength of the patch from the substrate.
1.9 Units—The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system are not necessarily exact equivalents; therefore, to ensure conformance with the standard, each system shall be used independently of the other, and values from the two systems shall not be combined.
1.10 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.11 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C125 Terminology Relating to Concrete and Concrete Aggregates
C1232 Terminology for Masonry
D883 Terminology Relating to Plastics
D3878 Terminology for Composite Materials
D5229/D5229M Test Method for Moisture Absorption Properties and Equilibrium Conditioning of Polymer Matrix Composite Materials
E6 Terminology Relating to Methods of Mechanical Testing
E122 Practice for Calculating Sample Size to Estimate, With Specified Precision, the Average for a Characteristic of a Lot or Process
ICS Number Code 91.100.40 (Products in fibre-reinforced cement)
UNSPSC Code 30111500(Concrete and mortars)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D7522 / D7522M-21, Standard Test Method for Pull-Off Strength for FRP Laminate Systems Bonded to Concrete or Masonry Substrates, ASTM International, West Conshohocken, PA, 2021, www.astm.orgBack to Top